In situ-grown hexagonal silicon nanocrystals in silicon carbide-based films
© Kim et al.; licensee Springer. 2012
Received: 14 July 2012
Accepted: 9 October 2012
Published: 21 November 2012
Silicon nanocrystals (Si-NCs) were grown in situ in carbide-based film using a plasma-enhanced chemical vapor deposition method. High-resolution transmission electron microscopy indicates that these nanocrystallites were embedded in an amorphous silicon carbide-based matrix. Electron diffraction pattern analyses revealed that the crystallites have a hexagonal-wurtzite silicon phase structure. The peak position of the photoluminescence can be controlled within a wavelength of 500 to 650 nm by adjusting the flow rate of the silane gas. We suggest that this phenomenon is attributed to the quantum confinement effect of hexagonal Si-NCs in silicon carbide-based film with a change in the sizes and emission states of the NCs.
Silicon-related low-dimensional structures such as Si nanocrystals (Si-NCs) have shown great potential in the development of next-generation devices. When Si-NCs are made smaller than the free-exciton Bohr radius of bulk Si, they behave as quantum dots[1–3] with various energy states that can be tuned using carrier confinement in all three dimensions. These quantum properties of Si-NCs have the greatest impact when they are embedded in a wide-gap dielectric matrix, the structure of which is quite intriguing in the field of Si optoelectronics and third-generation photovoltaics[4, 5].
Among such wide-gap dielectric matrices for optoelectronic and photovoltaic devices are Si carbide-based films. These films are considered to have one of the most promising top (window) layers due to a high transparency to photons absorbed by an underneath layer of Si-based junctions as well as to the conductive nature of the material. Moreover, when Si carbide-based film includes Si-NCs, the combination will certainly have further advantages. One such advantage is a lower barrier height caused by a lower bandgap of Si carbide (approximately 2.5 eV) compared to Si oxide (approximately 9 eV) and Si nitride (approximately 5.3 eV), which brings about an increased tunneling probability between Si-NCs[5–7]. Other advantages include the easy formation of minibands between Si-NCs and a higher Bloch carrier mobility[3, 8].
To fabricate Si-NCs in Si carbide-based dielectric matrix structures, high-temperature (T > 1,100°C) post-deposition annealing of a Si-containing amorphous dielectric film (i.e., Si oxide, Si nitride, and Si carbide) has been commonly used. However, this high-temperature process may pose a serious challenge in the development of a device fabrication process. In this regard, we have developed a method for the in situ fabrication of Si-NCs during the deposition of Si nitride-based matrices[10–12]. However, no attempt has yet been made to create a Si carbide-based matrix, which forms the motivation of this study.
Another interesting subject related to the formation of Si-NCs is the control of Si polytypes[13–15]. It is well known that Si crystallizes into a cubic-diamond structure under normal growth and treatment conditions. However, Si is also known to have several polytypes that are stable only at high pressure. Among these Si polytypes, hexagonal-wurtzite Si is important as it sometimes appears in stressed amorphous Si and has enhanced non-linear optical properties for novel optoelectronic applications[13–15].
In this study, we demonstrate the in situ formation of hexagonal Si-NCs during the preparation of a silicon carbide-based matrix film at 250°C. The optical gaps of the Si-NCs have been characterized using photoluminescence (PL). Finally, we discuss the size effect of hexagonal Si-NC on its quantum confinement of carriers.
Plasma-enhanced chemical vapor deposition (PECVD)[10, 12] with methane (CH4, >99.999%) and silane (Ar-diluted SiH4, >99.9999%) as the reactant gases has been employed to form a Si carbide-based dielectric film. Oxygen atoms are incorporated from the ambient environment, as we will see later. The total pressure and power of the plasma are 0.5 Torr and 5 W, respectively. The use of this low plasma power and highly diluted source gas is proven to be essential in the in situ formation of Si-NCs in amorphous Si and Si nitride-based matrices[10, 12]. A Si(100) wafer was employed as the sample substrate, whose temperature during deposition was fixed at 250°C. The CH4 flow rate was fixed at 10 sccm, while the SiH4 flow rate was varied from 10 to 60 sccm to modulate the growth rate of the film. This variation in the SiH4 flow rate controls the size of the Si-NCs. The size and crystallinity of the Si-NCs were characterized through high-resolution transmission electron microscopy (HRTEM) using a Tecnai G2 F20 instrument (FEI Co., Hillsboro, OR, USA) operated at 200 kV. To investigate the energy band of the Si-NCs, we conducted PL measurements at room temperature using a He-Cd (325 nm) laser for the excitation. The chemical composition of the matrix film was investigated using Fourier-transformed infrared spectroscopy (FTIR; IFS66V/S and HYPERION 3000, Bruker, Ettlingen, Germany).
Results and discussion
The growth mechanism of Si-NCs in a Si carbide-based film may be identical to the in situ formation of Si-NCs in amorphous Si and Si nitride-based matrix films[10, 12]. Namely, the key condition is the low rate of film growth, which can be acquired by low plasma power as well as by a high dilution of the source gas. Under optimum conditions, the Si nanoparticles are dispersedly formed in the matrix films during the film growth[12, 20, 21]. The Si nanoparticles formed are then transformed into nanocrystalline Si by hydrogen radical diffusion from the amorphous Si nanoparticles[10, 12]. It is then likely that the structure of the Si-NCs is influenced by their surrounding matrix at the moment of crystallization. Namely, one possible mechanism for the formation of hexagonal-wurtzitic Si-NCs is the surrounding oxygen and carbon atoms (network) inducing sufficient stresses on the nuclei[13, 15].
We suggest the third possibility, the quantum confinement effect, being the most likely origin of the PL emission. As we have seen in Figure 1a,c, the PL redshift with increasing SiH4 flow rate (Figure 3b) is accompanied by enlargement of the Si-NC size. This tendency between the PL energy versus Si-NC size d is consistent with the reported value based on the quantum confinement effect of A + B/d^ 2 with A = 1.475 eV and B = 38.5 (A is the bulk bandgap of the hexagonal crystal silicon, and B is the confinement parameter)[10, 13, 21], although further HRTEM observations are needed to determine the intermediate d values required for a more detailed analysis. Still, this A value is in reasonable agreement with the theoretical value of the direct-gap energy of approximately 1.48 eV by Joannopoulos and Cohen and the experimental value (PL gap energy) of approximately 1.45 both for hexagonal-wurtzite Si crystal.
The FTIR results of the Si-O peak intensity and PL spectra provide further support for the dominance of the quantum confinement effect. Figure 4 shows the relative FTIR absorption peak intensities of the Si-O stretching mode and the PL bandgap energy as a function of the SiH4 flow rate. As the SiH4 flow increases, the PL energy decreases while the Si-O mode intensity increases. Increasing the Si-O peak intensity means the increase of the oxygen content in the matrix, and it means the increase of the optical bandgap. The lowering of the PL energy, however, despite the increase of the oxygen content in the matrix, clearly indicates the dominance of the quantum confinement effect in determining the PL energy of the Si-NCs. We can therefore suggest that the hexagonal Si-NCs may have a tunable bandgap energy based on their size through the quantum confinement effect.
We investigated the in situ formation of Si-NCs during the growth of the surrounding Si carbide-based film through PECVD using methane (CH4) and silane (SiH4). No post-annealing process is necessary. The HRTEM measurements and PL results indicate the formation of Si-NCs with a hexagonal structure and good tunability of the optical bandgap under the growth conditions. The blueshift in the PL peak with a decreasing SiH4 flow rate can be attributed to the three-dimensional quantum confinement effect in the hexagonal Si-NCs. These results demonstrate the viable potential of this method for the fabrication of silicon-based third-generation photovoltaics.
The authors sincerely thank Dr. Hu Young Jeong (Graduate School of EEWS at KAIST) for conducting the electron diffraction analysis. This research was supported by the Research & Development Improvement Program for ETRI (project number 10041416) funded by MKE/KEIT and the R&D program of ETRI (11BF1300, Project Planning of Convergence System Components and Material Technology) in Korea.
- Pavesi L, Lockwood DJ: Silicon Photonics: Silicon Fundamentals for Photonic Applications. Heidelberg: Berlin; 2004.Google Scholar
- Walters RJ, Bourianoff GI, Atwater HA: Field-effect electroluminescence in silicon nanocrystals. Nature Material 2005, 4: 143–146. 10.1038/nmat1307View ArticleGoogle Scholar
- Jiang CW, Green MA: Silicon quantum dot superlattices: modeling of energy bands, densities of states, and mobilities for silicon tandem solar cell applications. J Appl Phys 2006, 99: 114902. 10.1063/1.2203394View ArticleGoogle Scholar
- Park N-M, Kim T-S, Park S-J: Band gap engineering of amorphous silicon quantum dots for light-emitting diodes. Appl Phys Lett 2001, 78: 2575–2577. 10.1063/1.1367277View ArticleGoogle Scholar
- Cho E-C, Park S, Hao X, Song D, Conibeer G, Park SC, Green MA: Silicon quantum dot/crystalline silicon solar cells. Nanotechnology 2008, 19: 245201. 10.1088/0957-4484/19/24/245201View ArticleGoogle Scholar
- Cheng Q, Xu S, Long J, Ostrikov K: Deterministic plasma-aided synthesis of high-quality nanoislanded nc-SiC films. Appl Phys Lett 2007, 90: 173112. 10.1063/1.2731728View ArticleGoogle Scholar
- Kurokawa Y, Tomita S, Miyajima S, Yamada A, Konagai M: Photoluminescence from silicon quantum dots in Si quantum dots/amorphous SiC superlattice. Jpn J Appl Phys 2007, 46: L833-L835. 10.1143/JJAP.46.L833View ArticleGoogle Scholar
- Song D, Cho E-C, Conibeer G, Flynn C, Huang Y, Green MA: Structural, electrical and photovoltaic characterization of Si nanocrystals embedded SiC matrix and Si nanocrystals/c-Si heterojunction devices. Sol Energy Mater Sol Cells 2008, 92: 474–481. 10.1016/j.solmat.2007.11.002View ArticleGoogle Scholar
- Wang YQ, Wang YG, Cao L, Cao ZX: High-efficiency visible photoluminescence from amorphous silicon nanoparticles embedded in silicon nitride. Appl Phys Lett 2003, 83: 3474–3476. 10.1063/1.1621462View ArticleGoogle Scholar
- Kim T-Y, Park N-M, Kim K-H, Sung GY, Ok Y-W, Seong T-Y, Choi C-J: Quantum confinement effect of silicon nanocrystals in situ grown in silicon nitride films. Appl Phys Lett 2004, 85: 5355–5357. 10.1063/1.1814429View ArticleGoogle Scholar
- Kim T-Y, Park N-M, Choi C-J, Huh C, Ahn C-G, Sung GY, You I-K, Suemitsu M: Effects of the hole tunneling barrier width on the electrical characteristic in silicon quantum dots light-emitting diodes. Jpn J Appl Phys 2011, 50: 04DG11. 10.1143/JJAP.50.04DG11View ArticleGoogle Scholar
- Kim T-Y, Park N-M, Choi C-J, Kim A, You I-K, Suemitsu M: Comparative study of silicon quantum dot formation in-situ grown with a gas mixture of SiH4+N2 and SiH4+NH3. J Korean Phys Soc 2011, 59: 308–311. 10.3938/jkps.59.308View ArticleGoogle Scholar
- Bandet J, Despax B, Caumont M: Vibrational and electronic properties of stabilized wurtzite-like silicon. J Phys D: Appl Phys 2002, 35: 234–239. 10.1088/0022-3727/35/3/311View ArticleGoogle Scholar
- Zhang Y, Iqbal Z, Vijayalakshmi S, Grebel H: Stable hexagonal-wurtzite silicon phase by laser ablation. Appl Phys Lett 1999, 75: 2758–2760. 10.1063/1.125140View ArticleGoogle Scholar
- Kumar KUM, Krishna MG: Chromium-induced nanocrystallization of a-Si thin films into the Wurtzite structure. J Nanomaterials 2008. 10.1155/ 736534Google Scholar
- Yeh C-Y, Lu ZW, Froyen S, Zunger A: Zinc-blende-wurtzite polytypism in semiconductors. Phys Rev B 1992, 46: 10086–10097. 10.1103/PhysRevB.46.10086View ArticleGoogle Scholar
- Kaneko T, Nemoto D, Horiguchi A, Miyakawa N: FTIR analysis of a-SiC:H films grown by plasma enhanced CVD. J Crystal Growth 2005, 275: e1097-e1101. 10.1016/j.jcrysgro.2004.11.128View ArticleGoogle Scholar
- Kim HY, Shao Q, Kim Y-H: Characterization of low-dielectric-constant SiOC thin films deposited by PECVD for interlayer dielectrics of multilevel interconnection. Surf Coat Technol 2003, 171: 39–45.View ArticleGoogle Scholar
- Lucovsky G, Niimi H: Remote plasma-assisted oxidation of SiC: a low temperature process for SiC–SiO2 interface formation that eliminates interfacial Si oxycarbide transition regions. J Phys Condens Matter 2004, 16: S1815-S1837. 10.1088/0953-8984/16/17/018View ArticleGoogle Scholar
- Edelberg E, Bergh S, Naone R, Hall M, Aydil ES: Luminescence from plasma deposited silicon films. J Appl Phys 1997, 81: 2410–2417. 10.1063/1.364247View ArticleGoogle Scholar
- Sung GY, Park N-M, Shin J-H, Kim K-H, Kim T-Y, Cho KS, Huh C: Physics and device structures of highly efficient silicon quantum dots based silicon nitride light-emitting diodes. IEEE J Sel Top Quant Electron 2006, 12: 1545–1555.View ArticleGoogle Scholar
- Wolkin MV, Jorne J, Fauchet PM, Allan G, Delerue C: Electronic states and luminescence in porous silicon quantum dots: the role of oxygen. Phys Revi Lett 1999, 82: 197–200. 10.1103/PhysRevLett.82.197View ArticleGoogle Scholar
- Nevin WA, Yamagishi H, Yamguchi M, Tawada Y: Emission of blue light from hydrogenated amorphous silicon carbide. Nature 1994, 368: 529–531. 10.1038/368529a0View ArticleGoogle Scholar
- Ma T, Xu J, Chen K, Du J, Li W, Huang X: Red-green-blue light emission from hydrogenated amorphous silicon carbide films prepared by using organic compound xylene as carbon source. Appl Phys Lett 1998, 72: 13–15. 10.1063/1.120631View ArticleGoogle Scholar
- Joannopoulos JD, Cohen ML: Electronic properties of complex crystalline and amorphous phases of Ge and Si. I. Density of states and band structures. Phys Rev B 1973, 7: 2644–2657. 10.1103/PhysRevB.7.2644View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.